1 Polish Journal of Environmental Studies Vol. 13, No. 6 (24), Original Research Fly Ash Zeolites as Sulfur Dioxide Adsorbents T. T. Suchecki 1,2 *, T. Wałek 3, M. Banasik 2 1 Research Center for Sustainable Materials Engineering, Institute of Multidisciplinary Research for Advanced Materials, Tohoku University, Katahira 2-1-1, Aoba-ku, Sendai , Japan 2 Laboratory of Toxicology and Risk Assessment, Institute of Coal Chemistry, Polish Academy of Sciences, ul. Sowińskiego 5, 44-1 Gliwice, Poland 3 Division of Environmental Management, Faculty of Organization and Management, Technical University of Silesia, ul. Roosevelta 26-28, 41-8 Zabrze, Poland Received: 29 December 23 Accepted: 1 June 24 Abstract Air protection technologies generate massive amounts of solid wastes, including fly ash (FA). Zeolite synthesis from FA seems to be an effective method for FA utilization. In addition, fly ash zeolites (FAZs) could be used for sulfur dioxide ( ). Since there is a lack of sufficient information about uptake on FAZs, we investigated this phenomenon in detail. Two commercially available zeolites, 3A and SM-27, and two FAZs, one manufactured by the authors and the other obtained from Kimura Chemical Plants, were used for tests. Our experiments confirmed that FAZs could be efficient adsorbents. Observed zero emission periods varied from 2-3 min for non-activated zeolites to 7-15 min for their thermally activated counterparts. The thermal activation of FAZs increased 2-3 times their capacity, resulting in up to 38 mg of /g of zeolitic material. Keywords: fly ash, zeolite, sulfur dioxide,. Introduction At present, fossil fuels are primary sources of energy in global as well as in most of the regional scales. Most air protection problems connected with stationary power generating plants, fueled by hard coal or lignite, are solved by the use of modern air protection technologies. However, these technologies generate massive amounts of solid wastes, e.g., gypsum from wet desulfurization units or fly ash (FA) separated from flue gases. In Poland, for example, every year more than four million tons of FA are produced in power and thermal plants, with 65% of this waste being utilized and 35% being stored in waste disposal sites . There are many possible methods of FA utilization and application. Production of cement or construction materials and civil engineering applications are the traditional *Corresponding author; fields of FA utilizations. Statistical information and many examples from Europe, USA, and Japan are available at the following websites: and Scheetz and Earle wrote an extensive overview of FA utilization in the aforementioned fields, dividing them into six groups: a. cement and concrete products, b. structural fillings and cover materials, c. waste solidification and stabilization, d. roadway and pavement constructions, e. lightweight aggregate materials production, and f. infiltration barrier construction and underground void filling . Horiuchi et al. presented effective ways of FA slurry use in underwater disposal, man-made island construction, and structural fills . Queralt et al. summarized the use of FA for ceramics manufacturing . There are also a number of possible FA applications outside of the construction industry. FA can be effectively used for
2 724 Suchecki T. T. et al. Table 1. Properties of employed zeolites. Manufacturer Name 3A zeolite SM-27 zeolite Kimura FAZ Our FAZ POCh S.A., Gliwice, Poland Alsi-Penta Zeolithe GmbH, Schwandorf, Germany Kimura Chemical Plants Co., Ltd., Amagasaki, Japan Authors Type Na-A ZSM-27 Phillipsite Na-P1 / Na-P a JCPDS No. b ND c ; Micropore diameter (nm) (.44 after dehydration) ; Structural change temperature ( C) 7 ND 2 25 Chemical formula Na 96 Al 96 Si 96 O H 2 O ND (K,Na) 2 (Si,Al) 8 O 16 4H 2 O Na Al Si O32 12H O; Na 3.6 Al 3.6 Si 12.4 O 32 14H 2 O a High-silica variety. b Joint Committee of Powder Diffraction Standard. c ND: no data provided by the manufacturer. the production of different types of zeolites, commercial grade mullite, glass-like materials for industrial applications, plastic and metal composite materials, and sorbents for waste management or waste stabilization and for agriculture purposes . Recently, many studies have been published about employing FA as a raw material for zeolite synthesis, although this process was demonstrated for the first time almost twenty years ago. Zeolites are manufactured in the process of hydrothermal treatment of FA. A class F power plant FA contains large quantities of silica oxide (~5%) and aluminum oxide (~25%). The zeolite synthesis occurs in the presence of sodium or potassium hydroxide at an appropriate time and temperature. The crystallization of various types of fly ash zeolites (FAZs) is a function of reaction time, temperature, ph, and concentrations of FA and the respective hydroxide. Usually, FA zeolitic process efficiency is 5-6%, but much lower values have also been reported. A literature search on FAZ syntheses indicates that the following types of zeolites have been identified thus far: faujasite [6, 7], Na-A , Na-P , Na-P1 [8-1], Na-X , P [7, 12], and phillipsite . In addition, mixtures of two different zeolites, analcime and sodalite , gobbinsite and Na-P1 , K-L and K-W , Na-A and Na-X , Na-P1 and analcime , Na- P1 and hydroxy-sodalite , Na-P1 and Na-X , and P and hydroxy-sodalite , or mixtures of three different zeolites, analcime, hydroxy-sodalite and tobermosite ; analcime, Na-P and gmelinite ; kalsilite, linde-f and tobermorite ; and Na-P1, analcime and gmelinite , were also reported. The aforementioned syntheses were conducted under batch regime in a laboratory scale. According to data provided by Donald W. Breck in his fundamental textbook on zeolites published in 1974, zeolites (KL, Na-A, Ca-A, and Na-X) of sulfur dioxide ( ) at low concentrations (several hundreds ppm) at 25 C ranges from 13 to 17 mg/g of zeolitic material . Since then, more experimental data for other types of zeolites have been published, e.g., approximately 38 mg /g of sillicalite , 128 and 19.2 mg /g of sillicalite S-115 and DAY, respectively , 267 mg /g of Na-Y . Few papers, however, have dealt with on FAZ. Srinivasan and Grutzeck demonstrated a relationship between drying condition of FAZ and . Their zeolites, dried in the air at 11 C, adsorb three times smaller amounts of than those dried in a microwave, i.e., 6-7 mg /g of analcime or sodalite zeolite. Querol et al. reported that KM and Na-P1 zeolites adsorb up to 2 mg of /g of zeolite, but much higher values were found for the following FAZs: Na-chabazite 1, 4A 3, and X 38 mg of /g . It should be noted that these researchers employed thermally activated zeolites. FAZs could be cost-effective sorbents for controlling emissions from industrial sources. The lack of information about uptake on FAZs, both thermally activated and not activated, encouraged us to further investigate this phenomenon. Experimental Procedures Zeolites Two commercially available zeolites, 3A and SM-27, and two FAZs, one manufactured by us and the other obtained from Kimura Chemical Plants Co., Ltd. (Amagasaki, Japan), were used for tests (Table 1). A detailed procedure of our FAZ manufacturing process have been described . Briefly, FA samples were collected from a dust chamber of an electrostatic precipitator of the 6th boiler of Łagisza Power Plant (Będzin, Poland) fueled by pulverized hard coal. FA (1 g/l of base solution) was added to 2. M NaOH solution. This reaction slurry was continuously mixed and kept at 8 C for 24 h. The zeolitic material produced was filtered, washed four times with distilled water, and then dried at 1 C for 6 h. A FAZ produced this way is referred in this paper as non-activated. In addition, activated forms of FAZs were generated by keeping the
3 Fly Ash Zeolites as Sulfur Dioxide necessary amounts of samples at 4 C for 1 h. The commercial zeolites were thermally activated using the same method. Both forms of zeolites were used for tests. Laboratory Set-Up The experimental set-up, shown in Fig. 1, consists of the following elements: and nitrogen gas cylinders, mass flow controllers (BETA-ERG, Sp. z o.o., Warsaw, Poland), a gas mixing chamber, a fixed-bed glass adsorber (~2 cm in length, 2.5 cm in diameter), and an infrared non-dispersive analyzer Rosemount 88 (Rosemount Analytical Inc., USA) with on-line recording. A desired gas mixture was directed to the upper part of the adsorber and flowed through the zeolite sample placed on a sintered glass shelf in the bottom part of the adsorber. The gases used, (1%) and nitrogen (99.99%), were purchased from MG Polska (Chorzów, Poland). Fig. 1. Schematic diagram of the experimental set-up. Procedure Gas flow rate and concentration were maintained at 6 L/h and 15 ppm, respectively. The relative proportions of and nitrogen were controlled with the mass flow controllers. First, gas was run through the adsorber bypass. Next, a zeolite sample (2. g) was placed into the adsorber. After the recording system of the analyzer was turned on, gas flow was switched from the bypass to the adsorber. After a run, gas was again directed to the bypass, the adsorber was opened, and the sample was collected. All experiments were conducted at room temperature. Results and Discussion Typical experimental results for the raw FA and our FAZ are shown in Fig. 2. was completely adsorbed on the zeolite bed in beginning periods of all runs. This period of zero emission time, called also the breakthrough time (tb), depends on employed material. It varied from 1 to 1 min for the raw FA and our FAZ, respectively. Next, outlet concentrations gradually increased up to the level of the inlet concentration. When the outlet concentration reached the inlet concentration, the bed became completely saturated with. The period between the beginning of the run and the bed saturation is called filling up time (tf). For calculations we used tf values that correspond to the time-point when the outlet concentration reached 95% of inlet concentration. The amount of adsorbed during the tb and the tf period is Ab and Af (mg of /g of zeolitic material), respectively. Results presented in Fig. 2 clearly show that our FAZ adsorbed several times more than the raw FA. 15 Raw Fly Ash Zeolitic Material 1 Inlet SO2 Concentration (15 ppm) 95% of Inlet Concentration (997 ppm) [SO2], ppm 5 5% of Inlet Concentration (52 ppm) tb tf tb tf Fig. 2. Breakthrough curves for the raw FA and our FAZ.
4 726 Suchecki T. T. et al. Af Ab tb tf Af Ab tb tf Ab & Af, mg /g zeolitic material Ab & Af, mg /g zeolitic material A SM-27 Our FAZ Kimura FAZ 3A SM-27 Kimura FAZ Our FAZ Fig. 3. Amounts of adsorbed (Ab and Af) on non-activated zeolites and their corresponding breakthrough (tb) and filling up (tf) times. Fig. 4. Amounts of adsorbed (Ab and Af) on activated zeolites and their corresponding breakthrough (tb) and filling up (tf) times. The observed relatively long -zero emission times of tested FAZs have important implications for technological applications of FA in flue gas control systems. FAZ as sorbent should have contact with flue gases for longer periods of time to be fully saturated by. This limitation means that a fluidized bed contactor should be employed; a fixed bed apparatus can also be considered. But any contact method of FAZ and flue gases needs more process and economic analysis. Two commercially available zeolites and two FAZs were employed for kinetic tests. In addition, necessary amounts of these zeolites were thermally activated and also used for experiments. The uptakes obtained from the breakthrough curves are shown in Figs. 3 and 4. Results of on non-activated zeolites are presented in Fig. 3. Ab values for investigated zeolites ranged from.5 to 2. mg of /g of zeolitic material, the latter value being for the FAZs. The tb values for increased in the following order: 3A < SM-27 < our FAZ < Kimura FAZ. The commercial zeolites, 3A and SM-27, exhibited similar Af values, approximately 2.5 mg of / g of zeolite. But marked differences in Af values existed among FAZs. Results of on activated zeolites are shown in Fig. 4. The activation process did not change the property of the 3A zeolite. For other zeolites substantial changes in properties were observed. Ab values were approximately three times higher for the FAZs and approximately two times bigger for the SM-27 as compared to their non-activated counterparts. The tb values for increased in the following order: 3A < SM-27 < Kimura FAZ < our FAZ (~ 15 min.). A similar trend was observed for Af values (except that the Af value for Kimura FAZ was much higher than that for our FAZ). Both FA and FAZs are very hydrophobic materials. The thermal activation of zeolites removes adsorbed water molecules at lower temperatures and structural water at higher temperatures as well. But structural changes of zeolites at higher temperatures can also extend their internal surface areas and, therefore, affect their properties. Our experimental data confirmed this. The 3A zeolite has a very stable structure up to 7 o C (Table 1). Therefore, no significant differences in uptake were observed for its non-activated or thermally activated type. A different behavior was observed for the tested FAZs and SM-27. Their structural changes occurred at 2 o C (Kimura) and 25 o C (our FAZ) as shown in Table 1. This phenomenon is responsible for the dramatic rise in uptakes with thermally activated FAZs. In conclusion, the results confirmed that FAZs could be used for. Observed zero emission periods varied from 2-3 min for non-activated zeolites, and from 7-15 min for thermally activated ones. Furthermore, the thermal activation of FAZs increased capacity 2-3 times (up to 38 mg of /g of FAZ). References 1. CENTRAL STATISTICAL OFFICE. Statistical Yearbook of the Republic of Poland, 22; Warsaw, Poland, SCHEETZ B.E., EARLE R. Utilization of fly ash. Curr. Opin. Solid State Mater. Sci. 3 (5), 51, HORIUCHI S., KAWAGUCHI M., YASUHARA K. Effective use of fly ash slurry as fill material. J. Hazard. Mater. 76 (2-3), 31, QUERALT I., QUEROL X., LÓPEZ-SOLER A., PLANA F. Use of coal fly ash for ceramics: a case study for a large Spanish power station. Fuel 76 (8), 787, IYER R.S., SCOTT J.A. Power station fly ash - a review of value-added utilization outside of the construction industry. Resour. Conser. Recycl. 31 (3), 217, CHANG H.-L., SHIH W.-H. A general method for the conversion of fly ash into zeolites as ion exchangers for cesium. Ind. Eng. Chem. Res. 37 (1), 71, INOE K., TSUNEMATSU S., YAMADA H. Manufacture of A-type zeolites. Zeolites 17 (3), 315, 1996.
5 Fly Ash Zeolites as Sulfur Dioxide QUEROL X., ALASTUEY A., LÓPEZ-SOLER A., PLANA F., ANDRÉS J.M., JUAN R., FERRER P., RUIZ C.R. A fast method for recycling fly ash: microwave-assisted zeolite synthesis. Environ. Sci. Technol. 31 (9), 2527, QUEROL X., PLANA F., ALASTUEY A., LÓPEZ-SOLER A. Synthesis of Na-zeolites from fly ash. Fuel 76 (8), 793, QUEROL X., UMAÑA J.C., PLANA F., ALASTUEY A., LOPEZ-SOLER A., MEDINACELI A., VALERO A., DOMINGO M.J., GARCIA-ROJO E. Synthesis of zeolites from fly ash at pilot plant scale. Examples of potential applications. Fuel 8 (6), 857, SRINIVASAN A., GRUTZECK M.W. The adsorbtion of by zeolites synthesized from fly ash. Environ. Sci. Technol. 33 (9), 1464, MURAYAMA N., YAMAMOTO H., SHIBATA J. Mechanism of zeolite synthesis from coal fly ash by alkali hydrothermal reaction. Int. J. Miner. Process. 64 (1), 1, MOUHTARIS T., CHARISTOS D., KANTIRANIS N., FILIPPIDIS A., KASSOLI-FOURNARAKI A., TSIRAM- BIDIS A. GIS-type zeolite synthesis from Greek lignite sulphocalcic fly ashes promoted by NaOH solutions. Microporous Mesoporous Mater. 61 (1-3), 57, BELARDI G., MASSIMILA S., PIGA L. Crystallization of K-L and K-W zeolites from fly-ash. Resour. Conser. Recycl. 24 (2), 167, GRUTZECK M.W., SIEMER D.D. Zeolites synthesized from class F fly ash and sodium aluminate slurry. J. Am. Ceram. Soc. 8 (9), 2449, HOLLMAN G.G., STEENBRUGGEN G., JANSSEN- JURKOVIČOVÁ M. A two-step process for the synthesis of zeolites from coal fly ash. Fuel 78 (1), 1225, BRECK D.W. Zeolite Molecular Sieves: Structure, Chemistry, and Use; John Wiley & Sons, Inc.: New York, DENG S.G., LIN Y.S. Sulfur dioxide sorption properties and thermal stability of hydrophobic zeolites. Ind. Eng. Chem. Res. 34 (11), 463, TANTET J., EIĆ M., DESAI R. Breakthrough study of the and separation of sulfur dioxide from wet gas using hydrophobic zeolites. Gas Sep. Purif. 9 (3), 213, GUPTA A., GAUR V., VERMA N. Breakthrough analysis for of sulfur-dioxide over zeolites. Chem. Eng. Process. 43 (1), 9, QUEROL X., MORENO N., UMAÑA J.C., ALASTUEY A., HERNÁNDEZ E., LÓPEZ-SOLER A., PLANA F. Synthesis of zeolites from coal fly ash: an overview. Int. J. Coal Geol. 5 (1-4), 413, WALEK T., IWATA H., OHYA H., SUCHECKI T. Synthesis of zeolites from Polish Class-F fly ash. Polish J. Environ. Stud. 9 (Suppl. I), 69, 2.